received: 27 October 2016 accepted: 26 January 2017 Published: 02 March 2017
Quantum spin Hall insulators in centrosymmetric thin films composed from topologically trivial BiTeI trilayers I. A. Nechaev1,2,3, S. V. Eremeev2,3,4,5, E. E. Krasovskii5,6,7, P. M. Echenique5,6 & E. V. Chulkov1,2,3,5,6 The quantum spin Hall insulators predicted ten years ago and now experimentally observed are instrumental for a break- through in nanoelectronics due to non-dissipative spin-polarized electron transport through their edges. For this transport to persist at normal conditions, the insulators should possess a sufficiently large band gap in a stable topological phase. Here, we theoretically show that quantum spin Hall insulators can be realized in ultra-thin films constructed from a trivial band insulator with strong spin-orbit coupling. The thinnest film with an inverted gap large enough for practical applications is a centrosymmetric sextuple layer built out of two inversely stacked noncentrosymmetric BiTeI trilayers. This nontrivial sextuple layer turns out to be the structure element of an artificially designed strong three-dimensional topological insulator Bi2Te2I2. We reveal general principles of how a topological insulator can be composed from the structure elements of the BiTeX family (X = I, Br, Cl), which opens new perspectives towards engineering of topological phases. Two-dimensional (2D) topological insulators (TIs)—a new electronic phase also referred to as a quantum spin Hall (QSH) insulator—are characterized by an absolute band gap induced by spin-orbit coupling (SOC) and helical gapless edge states inside the gap1. These states protected by time-reversal symmetry provide perfectly conducting spin-filtered channels, meeting the demands of low-power nanoelectronics and spintronics. The existence of such states as the fingerprint of a topologically non-trivial 2D insulator was first predicted in Refs 2,3. It was also suggested that the QSH effect can be observed in graphene, where SOC opens a gap at the two inequivalent Dirac points. This gap in graphene appears to be too small for practical use, so heavy-elements based analogs of graphene must be sought. Actually, the 2D materials with low-buckled honeycomb-lattice structures4–10—silicene, germanene, and stanene—possess a significantly larger SOC-induced gap at the Dirac points (up to ~0.1 eV in stanene), and the spin-polarized edge channels could be detected at easily accessible temperatures. However, the QSH effect in such systems has not been experimentally observed so far. Further effective enhancement of the SOC to make the gap larger can be realized by chemical functionalization of the above 2D materials11,12. Such a functionalization substantially enlarges the gap, in fact “destroying” the Dirac cones, and it may lead to a SOC-induced band inversion at the time reversal invariant momentum (TRIM) (normally at k = 0) with an absolute gap of several hundred meV at this momentum. If the band inversion occurs, the resulting 2D system is a 2D TI that should support the QSH effect12 similar to the inverted HgTe quantum wells predicted to be QSH insulators in ref. 13. It is important that this prediction has found experimental confirmation: In the inverted HgTe/CdTe and InAs/GaSb quantum wells14–16 the QSH effect was observed despite the very small gaps in these quantum wells, less than 10 meV. It has spurred a rising tide of theoretical
Centro de Física de Materiales CFM - MPC and Centro Mixto CSIC-UPV/EHU, 20018 San Sebastián/Donostia, Spain. Tomsk State University, 634050, Tomsk, Russia. 3Saint Petersburg State University, 198504, Saint Petersburg, Russia. 4Institute of Strength Physics and Materials Science, 634055, Tomsk, Russia. 5Donostia International Physics Center, 20018 San Sebastián/Donostia, Spain. 6Departamento de Física de Materiales UPV/EHU, Facultad de Ciencias Químicas, UPV/EHU, Apdo. 1072, 20080 San Sebastián/Donostia, Spain. 7IKERBASQUE, Basque Foundation for Science, 48013, Bilbao, Spain. Correspondence and requests for materials should be addressed to I.A.N. (email: [email protected]
Scientific Reports | 7:43666 | DOI: 10.1038/srep43666
www.nature.com/scientificreports/ propositions of different 2D TIs with honeycomb- or square-lattice structures and a large inverted gap enabling room-temperature operating17. Ab initio approaches to electronic structure, especially those based on the density functional theory (DFT), have become a powerful tool to search for new materials with unique properties. At the same time, the effective models that proved indispensable in predicting the QSH effect in graphene-like systems and quantum wells are currently widely used to analyze the effect of strain, quantum confinement, and external fields in 2D TIs, i.e., to solve the problems that presently are not accessible with ab initio methods. Thus, to efficiently model the nanoelectronics and spintronics devices, the microscopic methodology must be bridged with the effective Hamiltonian approach based on symmetry considerations and on the k·p perturbation theory. With a few exceptions, none of the theoretically proposed 2D materials has been hitherto fabricated17. Thus, the intensive search of robust and easily fabricated materials remains to be actual. In particular, it was suggested that 2D TIs can be produced from a thin film of layered 3D (three-dimensional) TIs of the Bi2Se3 family, where the hybridization between the opposite surfaces of the film opens a gap at the Dirac point (DP). Depending on film thickness, the 2D system may “oscillate” between band insulator and QSH insulator as was predicted by the 4-band effective k·p model (see refs 18,19). The thinnest known topologically nontrivial film consists of at least two structural elements—quintuple or septuple layers20. Besides the studies on the thin films of 3D TIs, recently it was heuristically suggested that a 3D TI can be constructed artificially via stacking 2D bilayers that are topologically trivial21. It encourages our search for 2D TIs built out of trivial band-insulator constituents. These constituents should have strong spin-orbit coupling (SOC), and prospective candidates are bismuth tellurohalides BiTeX with X = I, Br, and Cl, among which the polar semiconductor BiTeI demonstrates the strongest spin-orbit coupling providing the biggest known Rashba spin-splitting of bulk and surface states22,23. The structure element of BiTeI is a trilayer (TL) with the I-Bi-Te stacking. A single TL that possesses the Rashba spin-split band structure24 can be grown epitaxially on a suitable substrate or be easily exfoliated from the bulk BiTeI, where the adjacent TLs couple through a weak van-der-Waals (vdW) interaction. The samples of BiTeI always contain a large number of randomly distributed bulk stacking faults, which leads to a mixture of terminations at the surface, as experimentally observed in refs 25–30. This implies that adjacent TLs may have different sequence order along the hexagonal z axis. Here, based on DFT calculations we demonstrate that a centrosymmetric sextuple layer (SL) constructed from two BiTeI TLs with facing Te-layer sides and a typical vdW spacing is a 2D TI with the gap of 70 meV at Γ. The vdW interaction between these TLs is crucial to realize such a QSH insulator phase: The SL becomes topologically trivial with increasing the vdW spacing by 5% only. We consider the nontrivial SL as a structure element, a repetition of which along the z axis results in thin films that are found to “oscillate” between trivial and nontrivial phases with the number of SLs. The corresponding bulk system composed of SLs turns out to be a strong 3D TI (hereafter referred to as Bi 2Te 2I 2). It is energetically unfavourable by only 0.5 meV compared with the non-centrosymmetric BiTeI. This makes it plausible to suppose that crystals of BiTeI grown by the Bridgman method already contain the desired SLs, and that the alternative stacking can be experimentally observed and controllably manufactured. To describe the low-energy properties of Bi2Te2I2 and its films, we derive four-band k·p Hamiltonians from the ab initio wave functions. They are similar to the Hamiltonians constructed for Bi2Se3 -family 3D TIs and their thin films18,31,32. For a more accurate description of the SL, we derive an eight-band Hamiltonian that involves Rashba-split valence and conduction bands of the stand-alone TLs. We thus demonstrate that due to the bonding-antibonding splitting the inversion occurs between one of the Te-related valence bands and one of the conduction bands formed by Bi orbitals. The proposed materials illustrate the effectiveness of the new way to design 2D TIs from trivial band insulators with giant-Rashba spit bands for room-temperature operating.
Figure 1(a–c) show the band structure of 1 and 5 SLs and the bulk crystal of Bi2Te2I2 obtained with the extended linearized augmented plane wave (ELAPW) method33 within the local density approximation (LDA) for the exchange-correlation functional and with the use of the full potential scheme of ref. 34. (Details on the equilibrium bulk atomic structure, the bulk-truncated slab geometry of the related thin films, and the calculations performed can be found in Supplementary Note 1.) The 1SL film is constructed from two BiTeI trilayers with facing Te-layer sides, Fig. 1(d). It is noteworthy that the band structure of this film with the gap of 56 meV (70 meV in the relaxed geometry, see Supplementary Fig. 1) differs substantially from that of its constituents (cf. Supplementary Fig. 2): there is no trace of Rashba-type split bands. The band structure of the 5SL film exhibits a gapless Dirac state residing in the band gap of 151 meV, see Fig. 1(b) and Supplementary Fig. 3. This is a signature of the topological character of the respective bulk band structure (Fig. 1(c)), which has an inverted gap of 234 meV at Γand the fundamental gap of 169 meV in the Γ–A line close to the A point. As seen in Fig. 2(a), the Dirac surface state almost completely resides within the outer SL. Moreover, this state is localized stronger than the Dirac state of TIs like Bi2Te3, since 70% of its weight falls in the outermost half of the SL, i.e., in the surface BiTeI TL (see also Fig. 1(e)). The spin texture of the Dirac state is illustrated in Fig. 2(b) and (c), which show spin-resolved constant energy contours for the lower and upper cones of the Dirac surface state. Apart from the in-plane polarization – clockwise above the DP and counterclockwise below it, both contours also have an out-of-plane spin component, which is an intrinsic feature of the hexagonal surface. However, in this case Sz is extremely small and varies in the range of ≈±0.01. As has been shown for the Dirac state in Bi2Se3 both experimentally and theoretically35–39, the spin textures of px, py, and pz orbitals are remarkably different, which leads to the dependence of the spin polarization of photoelectrons on the polarization of light. The spin texture provided by pz orbitals has clockwise (counterclockwise) chirality for the upper (lower) cone, while the projections of the total spin on px and py orbitals are not chiral, Scientific Reports | 7:43666 | DOI: 10.1038/srep43666
Figure 1. Ab initio calculations for Bi2Te2I2. LDA band structure (black curves) of 1SL (a) and 5SL (b) films as well as the bulk crystal (c) of Bi2Te2I2. Red curves correspond to the eigenvalues E(k) of the model four-band Hamiltonian. Atomic layers maximally contributing to the valence and the conduction band at the center of the 2D Brillouin zone in the case of the Bi2Te2I2 films of different thickness are indicated in graph (e) by green and red bars, respectively. The dependence of the model Hamiltonian parameters on the number of SLs is presented in graphs (g,h). The atomic structure of the bulk Bi2Te2I2 (unit cell) and its 1SL film (d) with the corresponding 3D and 2D Brillouin zone (f) are also shown.
and their spins are opposite to each other. Similar spin-orbital texture we find in the Bi2Te2I2, see Fig. 2(d–f) for the upper Dirac cone (for the lower Dirac cone, the coupling of spin and orbital textures is opposite, not shown). As can be seen, the spin orientations for px and py projections are antiparallel at each k|| point, whereas the spin orientation of pz projection coincides with the total spin. It is noteworthy that similar spin-orbital texture has been observed for the spin-polarized Rashba state in BiTeI40. For the Te-terminated surface, it was found that the outer Rashba branch demonstrates the same spin Scientific Reports | 7:43666 | DOI: 10.1038/srep43666
Figure 2. Spin-orbital texture of the surface state. (a) Spatial localization of the topological surface state as a function of z, where z = 0 corresponds to the surface plane for Bi2Te2I2 and Bi2Te2. Spin-resolved constant energy contours are taken at 75 meV above (b) and at 50 meV below (c) the Dirac point (DP). Black arrows adjacent to the contours denote the in-plane spin component S||; the out-of-plane spin component Sz is indicated by the color in contour, with red and blue corresponding to positive and negative values, respectively. Projections of the total spin for upper Dirac cone, shown in panel (b), on the px (d), py (e), and pz (f) orbitals.
orientations for px, py, and pz projections as those for the upper Dirac cone in Bi2Te2I2, and the inner Rashba branch has opposite texture, i.e., the same as in the lower cone. Because the surface of the Bi2Te2I2 slab has iodine termination and its spin-texture is reversed due to the opposite orientation of the z axis, the spin-orbit texture of the upper (lower) Dirac cone in Bi2Te2I2 is the same as the texture of the inner (outer) Rashba branch in BiTeI. To construct a simple effective k·p model for the centrosymmetric Bi2Te2I2 we derive a model Hamiltonian of a desired dimension and accurate up to the second order in k from the LDA spinor wave functions Ψn↑(↓) of the doubly degenerate bands En found at k = 0 (see Supplementary Note 2 and ref. 41 for details). The subscripts ↑ or ↓ in Ψn↑(↓) refer to the z-component of the total angular momentum J = L + S in the atomic sphere that has the largest weight in the n-th band, see Fig. 1(e). The Hamiltonian is constructed in terms of the matrix elements42 πn ↑ (↓) m↑ (↓) = Ψn ↑ (↓) π Ψm↑ (↓) of the velocity operator π = − i∇ + [σ × ∇V ]/4m0 c 2, where n and m run over the relativistic bands (from semi-core levels up to high-lying unoccupied bands). Here, σ is the vector of the Pauli matrices, and V(r) is the crystal potential. bulk For the bulk Bi2Te2I2, in the basis of the two valence bands Ψvbulk ↑ (↓) and two conduction bands Ψc↑ (↓) , our ab initio four-band Hamiltonian reads: bulk Hkp = C τ 0σ 0 + M τ z σ 0
−V τ x (σ x k y − σ y k x ) − V z τ y σ 0kz , C z kz2
M z kz2
, k = kx2 + k y2, and bulk of Hkp is presented
where C = C 0 + the direct matrix product of the + C k , M = M0 + +Mk Pauli matrices τ and σ is implied (the explicit matrix form in Supplementary Note 3). Note that this Hamiltonian is the same (to within a unitary transformation) as that constructed for Bi2Se3 in ref. 31 within the theory of invariants. The matrices τ and σ in Eq. (1) have different meaning: τ operates in the valence-conduction band space, while σ refers to the total angular momentum J. The parameters in Eq. (1) obtained within the LDA are: C0 = 0.03 eV, Cz = 0.13 a.u., C|| = 4.19 a.u., M0 = −0.12 eV, M z = 1.35 a.u., M || = 5.88 a.u., V || = 0 .52 a.u., and V z = 0 .13 a.u. (we use Rydberg atomic units: = 2m0 = e 2/2 = 1). Since the basis functions explicitly refer to the valence and conduction bands rather than to atomic orbitals, the parameter M0 that defines the band gap at k = 0 is negative and does not change sign upon
Scientific Reports | 7:43666 | DOI: 10.1038/srep43666
Figure 3. Band structure of the 1SL Bi2Te2I2 film with different van-der-Waals spacing. The expansion of the spacing is 10% (b), 40% (c), 100% (d), 200% (e), 1100% (f) as indicated in percents of the bulk value (a). The spectra provided by the 4-band (red lines) and 8-band (blue lines) k·p models are presented in comparison with the LDA bands (black lines). Light green lines show the results of the 36-band Hamiltonian to demonstrate the convergence with respect to the size of the basis set. moving from the topologically non-trivial insulator to the trivial one. The eigenvalues E(k) of the Hamiltonian (1) with the above parameters are shown in Fig. 1(c) by red lines, nicely reproducing the LDA curves over a quite large k-region and providing an absolute gap in the k·p spectrum. Moreover, these parameters reflect the band inversion and meet the condition of the existence of topological surface states (see, e.g., ref. 43) in accord with the ℤ2 topological invariant ν3D = 1 obtained from the parities of the bulk LDA wave functions at the TRIM points44. Actually, the diagonal dispersion term Mz(||) is positive, and it is larger than the electron-hole asymmetry: |Cz(||)|